Research Article  Open Access
HsuanChung Wu, ShengHong Li, SyuanWei Lin, "Effect of Fe Concentration on FeDoped Anatase TiO_{2} from GGA + U Calculations", International Journal of Photoenergy, vol. 2012, Article ID 823498, 6 pages, 2012. https://doi.org/10.1155/2012/823498
Effect of Fe Concentration on FeDoped Anatase TiO_{2} from GGA + U Calculations
Abstract
To comprehend the photocatalytic mechanisms of anatase O_{2} with various concentrations of Fe, this study performed first principles calculations based on density functional theory with Hubbard U onsite correction to evaluate the crystal structure, impurity formation energy, and electronic structure. We adopted the effective Hubbard U values of 8.47 eV for Ti 3d and 6.4 eV for Fe 3d. The calculations show that higher concentrations of Fe are easily formed in anatase TiO_{2} due to a reduction in the formation energy. The band gap of Fedoped TiO_{2} decreases Fe doping level increases as a result of the overlap among the Fe 3d, Ti 3d, and O 2p states, which enhances photocatalytic activity in the visible light region. Additionally, a broadening of the valence band and Fe impurity states within the band gap might also contribute to the photocatalytic activity.
1. Introduction
The increase in global pollution has led researchers to search for new techniques and materials to promote environmental protection. Since Fujishima and Honda’s report in 1972 [1], the unique properties of have attracted considerable attention in the fields of air and water purification, hydrogen production, and dyesensitized solar cells. Anatase also has a wide band gap capable of only absorbing ultraviolet (UV) light (≤387 nm). UV light accounts for a small fraction (~5%) of the available solar energy; therefore, the utilization of solar energy is low. To improve the photocatalysis of , determining how to expand the optical absorption into the visible light region (~45%) has become a topic of considerable interest among researchers.
Considerable research has gone into modifying the band gap of . One of the most effective methods involves doping crystals with impurities including transition metals, such as V [2], Mo [3], Fe [4–6], Co [7, 8], Pt [9], Au [10], and nonmetals such as N [11, 12], F [13], P [14], S [15]. Among these impurity elements, the radius of (0.64 Å) is similar to that of (0.68 Å) and is therefore easily incorporated into the crystal [16]. In addition, the dopant can serve as a charge trap, impeding the electronhole combination rate and enhancing photocatalysis within a range suitable to the concentration of the dopant [17]. Fe is considered an appropriate candidate element and has been widely studied [18–25]. Zhang et al. [18] prepared Fedoped mesoporous thin films and suggested that the doped Fe forms ions, which could play a role as or traps, thereby reducing the / pair recombination rate. Wang et al. [19] reported that the band gap of Fedoped thin films decreased from 3.29 to 2.83 eV with an increase in the content from 0 to 25 wt%. The decrease in unit cell volume indicates that replaced in the lattice, forming a solid solution. Some experimental results [20, 21] have found that Fe doping in could narrow the band gap of , thereby increasing the efficiency of the photocatalysis in the visible range. Yalçin et al. [22] performed calculations based on density function theory (DFT) to characterize the influence of Fe^{3+} doping on the electronic and structural properties of . The results indicate that the visible light activity in doped is due to the introduction of additional electronic states within the band gap.
Recently, firstprinciples calculations were conducted for Fedoped , but these have been restricted to a single concentration of Fe [23–25]. To the best of our knowledge, few of these studies have focused on the photocatalytic mechanisms of Fedoped anatase with different Fe concentrations. Additionally, most theoretical calculations have greatly underestimated the band gap of due to the adoption of the conventional DFT method, which is known to include an insufficient description of the onsite Coulomb interaction between electrons occupying the Ti 3d orbitals. This study performed firstprinciples calculations using the generalized gradient approximation + Hubbard U (GGA + U) approach to investigate the crystal structure, formation energy, and electronic structure of anatase . Various concentrations of Fe, , and 0.1875 (2.08, 4.17, and 6.25 at.%), were analyzed.
2. Calculation Models and Methods
Anatase has a tetragonal structure with lattice parameters Å, c = 9.486 Å. To calculate various concentrations of Fe, a 2 × 2 × 1 supercell was constructed with 16 Ti and 32 O atoms, as shown in Figure 1(a). The calculations for the doping system were conducted for the 2 × 2 × 1 supercell containing one, two, and three Fe atoms in the substitutional sites of the Ti atoms, as shown in Figures 1(b)–1(d), which correspond to the Fe concentrations of 2.08, 4.17, and 6.25 at.%, respectively.
(a)
(b)
(c)
(d)
Firstprinciples calculations were performed using the CASTEP module [26] in Materials Studio 5.0 developed by Accelrys Software Inc. Electronion interactions were modeled using ultrasoft pseudopotentials in the Vanderbilt form [27]. The valence configurations of the atoms were for Ti, for O, and for Fe. The wave functions of the valence electrons were expanded through a plane wave basisset and the cutoff energy was selected as 400 eV. The MonkhorstPack scheme [28] Kpoints grid sampling was set at 4 × 4 × 3 (less than 0.04 Å^{−1}) in the supercells. The convergence threshold for selfconsistent iterations was set at 5 × 10^{−6 }eV. The lattice parameters and atomic positions for each supercell system were first optimized using the generalized gradient approximation (GGA) together with the method introduced by Wu and Cohen [29]. The optimization parameters were set as follows: energy change = 9 × 10^{−5 }eV/atom, maximum force = 0.09 eV/Å, maximum stress = 0.09 GPa, and maximum displacement tolerance = 0.009 Å. To describe the electronic structures more accurately, the GGA + U method was adopted with the strong onsite Coulomb repulsion among the localized Ti 3d electrons described according to the following formalism [30, 31]: where denotes the spin () polarized onsite density matrix. The spherically averaged Hubbard parameter describes the increase in energy caused by the placement of an additional electron at a particular site, and the parameter (1 eV) represents the screened exchange energy. The effective Hubbard parameter , which accounts for the onsite Coulomb repulsion for each affected orbital, is the only external parameter required for this approach.
3. Results and Discussion
3.1. Structural Optimization
Table 1 summarizes the optimized lattice parameters, average bond lengths, and differences in volume, obtained from structure optimization. The optimized lattice parameters, a = b = 3.778 Å, and c = 9.549 Å, for pure anatase are in good agreement with the experimental values of a = b = 3.782 Å and c = 9.502 Å [32], indicating that our calculations are reliable. In anatase , each Ti atom is bonded to its four nearest and two second nearest oxygen neighbors. Average bond lengths are represented as Ti–O^{1st} and Ti–O^{2nd}. With the same concentration of Fe, all of the Fe–O bond lengths are shorter than those of Ti–O. Therefore, the volume decreases with an increase in Fe concentration, which is consistent with the experimental results [33]. This indicates that Fe doping causes a contraction in the overall volume, which may be the result of the difference in the radii of the ions: 64 pm for and 68 pm for .

3.2. Hubbard U Parameter
The GGA + U approach uses an intraatomic electronelectron interaction for onsite correction to describe systems with localized d and f electrons, capable of producing a more optimal band gap. Determining an appropriate Hubbard parameter is necessary in GGA + U calculations to correctly interpret the intraatomic electron correlation. As shown in Figure 2, for anatase , the band gap widens with an increase in the effective Hubbard of Ti 3d. The band gap was widened by increasing from 2 to 8 eV. Here, the onsite Coulomb interaction was = 8.47 eV for Ti 3d using the GGA + U approach and the calculated band gap of pure anatase is 3.21 eV, which is close to the experimental value of 3.2 eV. Using the same method, the = 6.4 eV of Fe 3d was determined by fitting the band gap of (2.2 eV).
3.3. Formation Energy
To examine the relative stability of doped with various concentrations of Fe, the defect formation energies were calculated according to the following formula: Here, (Fedoped) and (pure) are the total energies of Fedoped and pure ; is the number of substitutional Fe atoms; and represent the chemical potentials of the Fe and Ti atoms, respectively. The formation energy depends on the growth conditions, which can be Tirich or Orich. For , and satisfy the relationship + 2 = . Under the Orich growth condition, is determined by the total energy of an O_{2} molecule () and is determined by the formula − 2 . Under the Tirich growth condition, is the energy of one Ti atom in bulk Ti and is determined by /2. The values of are −1601.80 and −1592.61 eV under the Orich and Tirich, respectively. is the energy of one Fe atom in bulk Fe, and the calculated value is −856.33 eV. Table 2 summarizes the calculated formation energies for doped with various concentrations of Fe. It should be noted that the smaller the value is, the easier it is to incorporate impurities into the supercell. The formation energy of Fedoped is reduced to a greater degree under Orich conditions than under the Tirich conditions, indicating that the incorporation of Fe into at the site of the Ti atom is favorable. In addition, the formation energies decrease with an increase in Fe concentration under Orich conditions, suggesting that higher concentrations of Fe facilitate the synthesis of Fedoped anatase .

3.4. Electronic Structure
Figure 3 indicates the total density of states (TDOS), and the projected density of states (PDOS) to investigate the electronic properties of Fedoped anatase . The zeropoint energy is taken as the Fermi level. The band gap () of pure anatase is 3.21 eV, as shown in Figure 3(a), and is consistent with the experimental value of 3.2 eV. In pure anatase , the valence band (VB) mainly comprises O 2p states with a small number of Ti 3d states, while the conduction band (CB) comprises Ti 3d states with a small number of O 2p states. This indicates that there exists a little covalence bond character between Ti and O atoms. The valence band of has a large bandwidth () of approximately 4.63 eV, showing a strong delocalization among the O 2p electrons. At 2.08 at.% (Fe concentration) from Figure 3(b), we observe Fe 3d impurity states in the band gap ranging from 1.74 eV above the valence band maximum (VBM) to 0.52 eV below the conduction band minimum (CBM). The electrons in the VB can be excited to localized impurity states within the band gap and subsequently to the CB through the absorption of visible light. In addition, the substitutional Fe atom only transfers 3 electrons to the surrounding O atoms, which leads to unfilled O 2p orbitals and an electron remaining in the ion as shown in Figure 4. At 4.17 at.% (Figure 3(c)), the overlap of Fe 3d, Ti 3d, and O 2p bands near the CB results in a decrease in the CBM. Therefore, the band gap of Fedoped at 4.17 at.% narrows to 2.70. From 4.17 at.% to 6.25 at.% (Figure 3(d)), the CBM continuously moves toward the Fermi level and hybridization among Fe 3d, Ti 3d, and O 2p near the Fermi energy level also occur, resulting in a reduced band gap. Figure 5 shows the relationships between and and Fe concentration. decreases with an increase in the Fe doping level, which is similar to other experimental results [18, 19]. It also reveals that the decrease in from 2.08 at.% to 6.25 at.% is more obvious than that from 0 to 2.08 at.%. increases with an increase in Fe concentration due to the contribution from the lower Fe 3d band, which benefits the hole mobility in VB. As a result, the electron transition energy from the valence band to the conduction band decreases as a result of Fedoping, which may induce a red shift at the edge of the optical absorption range. In addition, the valence band was found to broaden after Fe was incorporated into due to the contribution from the lower Fe 3d states. broadens with an increase in Fe concentration. The wider valence band results in an increase in the mobility of the photogenerated electronhole pair. In this manner, both the narrowing of the band gap and the increased mobility of the photogenerated carriers can improve the photocatalytic activity under visible light.
(a)
(b)
(c)
(d)
4. Conclusions
This study used the GGA + U method to investigate the influence of doping concentration on the crystal structure, impurity formation energy, and electronic properties of Fedoped anatase . We adopted the effective Hubbard U values, 8.47 eV for Ti 3d and 6.4 eV for Fe 3d, to accurately determine the band gap in the experiments. The calculated results imply that higher concentrations of Fe facilitate the formation of anatase . In addition, doping anatase with Fe can effectively narrow the band gap, thereby increasing photocatalytic activity in the visible light region and the trend of band gap decreases with an increase in Fe concentration. Both the broadening of the valence band and Fe impurity states within the band gap might also enhance photocatalytic activity.
Acknowledgments
This work was supported by the National Science Council in Taiwan (NSC 1002221E131017), for which the authors are grateful. They also acknowledge the National Center for Highperformance Computing for computer time and the use of its facilities.
References
 A. Fujishima and K. Honda, “Electrochemical photolysis of water at a semiconductor electrode,” Nature, vol. 238, no. 5358, pp. 37–38, 1972. View at: Publisher Site  Google Scholar
 I. Tsuyumoto and K. Nawa, “Thermochromism of vanadiumtitanium oxide prepared from peroxovanadate and peroxotitanate,” Journal of Materials Science, vol. 43, no. 3, pp. 985–988, 2008. View at: Publisher Site  Google Scholar
 Y. K. Du, Y. Q. Gan, P. Yang, F. Zhao, N. P. Hua, and L. Jiang, “Improvement in the heatinduced hydrophilicity of TiO_{2} thin films by doping Mo(VI) ions,” Thin Solid Films, vol. 491, no. 12, pp. 133–136, 2005. View at: Publisher Site  Google Scholar
 H. Yamashita, M. Harada, J. Misaka, M. Takeuchi, B. Neppolian, and M. Anpo, “Photocatalytic degradation of organic compounds diluted in water using visible lightresponsive metal ionimplanted TiO_{2} catalysts: Fe ionimplanted TiO_{2},” Catalysis Today, vol. 84, no. 34, pp. 191–196, 2003. View at: Publisher Site  Google Scholar
 S. Zhu, T. Shi, W. Liu et al., “Direct determination of local structure around Fe in anatase TiO_{2},” Physica B, vol. 396, no. 12, pp. 177–180, 2007. View at: Publisher Site  Google Scholar
 K. Naeem and F. Ouyang, “Preparation of Fe^{3+}doped TiO_{2} nanoparticles and its photocatalytic activity under UV light,” Physica B, vol. 405, no. 1, pp. 221–226, 2010. View at: Publisher Site  Google Scholar
 M. Subramanian, S. Vijayalakshmi, S. Venkataraj, and R. Jayavel, “Effect of cobalt doping on the structural and optical properties of TiO_{2} films prepared by solgel process,” Thin Solid Films, vol. 516, no. 12, pp. 3776–3782, 2008. View at: Publisher Site  Google Scholar
 D. Sarkar, C. K. Ghosh, U. N. Maiti, and K. K. Chattopadhyay, “Effect of spin polarization on the optical properties of Codoped TiO_{2} thin films,” Physica B, vol. 406, no. 8, pp. 1429–1435, 2011. View at: Publisher Site  Google Scholar
 X. Wenbin, D. Shurong, W. Demiao, and R. Gaochao, “Investigation of microstructure evolution in Ptdoped TiO_{2} thin films deposited by rf magnetron sputtering,” Physica B, vol. 403, no. 17, pp. 2698–2701, 2008. View at: Publisher Site  Google Scholar
 M. Zhou, J. Zhang, B. Cheng, and H. Yu, “Enhancement of visiblelight photocatalytic activity of mesoporous AuTiO_{2} nanocomposites by surface plasmon resonance,” International Journal of Photoenergy, vol. 2012, Article ID 532843, 10 pages, 2012. View at: Google Scholar
 H. Fu, G. Shang, S. Yang, and T. Xu, “Mechanistic study of visiblelightinduced photodegradation of 4chlorophenol by ${\text{TiO}}_{2x}{\text{N}}_{x}$ ($0.021<x<0.049$) with low nitrogen concentration,” International Journal of Photoenergy, vol. 2012, Article ID 759306, 9 pages, 2012. View at: Google Scholar
 J. Qian, G. Cui, M. Jing, Y. Wang, M. Zhang, and J. Yang, “Hydrothermal synthesis of nitrogendoped titanium dioxide and evaluation of its visible light photocatalytic activity,” International Journal of Photoenergy, vol. 2012, Article ID 198497, 6 pages, 2012. View at: Google Scholar
 M. V. Dozzi, S. Livraghi, E. Giamello, and E. Selli, “Photocatalytic activity of S and Fdoped TiO_{2} in formic acid mineralization,” Photochemical & Photobiological Sciences, vol. 10, no. 3, pp. 343–349, 2011. View at: Google Scholar
 Y. Lv, L. Yu, H. Huang, H. Liu, and Y. Feng, “Preparation, characterization of Pdoped TiO_{2} nanoparticles and their excellent photocatalystic properties under the solar light irradiation,” Journal of Alloys and Compounds, vol. 488, no. 1, pp. 314–319, 2009. View at: Publisher Site  Google Scholar
 T. Umebayashi, T. Yamaki, H. Itoh, and K. Asai, “Band gap narrowing of titanium dioxide by sulfur doping,” Applied Physics Letters, vol. 81, no. 3, pp. 454–456, 2002. View at: Publisher Site  Google Scholar
 M. Zhou, J. Yu, and B. Cheng, “Effects of Fedoping on the photocatalytic activity of mesoporous TiO_{2} powders prepared by an ultrasonic method,” Journal of Hazardous Materials, vol. 137, no. 3, pp. 1838–1847, 2006. View at: Publisher Site  Google Scholar
 J. Zhang, Y. Wu, M. Xing, S. A. K. Leghari, and S. Sajjad, “Development of modified N doped TiO_{2} photocatalyst with metals, nonmetals and metal oxides,” Energy and Environmental Science, vol. 3, no. 6, pp. 715–726, 2010. View at: Publisher Site  Google Scholar
 Y. Zhang, Y. Shen, F. Gu, M. Wu, Y. Xie, and J. Zhang, “Influence of Fe ions in characteristics and optical properties of mesoporous titanium oxide thin films,” Applied Surface Science, vol. 256, no. 1, pp. 85–89, 2009. View at: Publisher Site  Google Scholar
 M. C. Wang, H. J. Lin, and T. S. Yang, “Characteristics and optical properties of iron ion (Fe^{3+})doped titanium oxide thin films prepared by a solgel spin coating,” Journal of Alloys and Compounds, vol. 473, no. 12, pp. 394–400, 2009. View at: Publisher Site  Google Scholar
 W. Weng, M. Ma, P. Du et al., “Superhydrophilic Fe doped titanium dioxide thin films prepared by a spray pyrolysis deposition,” Surface and Coatings Technology, vol. 198, no. 1–3, pp. 340–344, 2005. View at: Publisher Site  Google Scholar
 J. B. Naceur, R. Mechiakh, F. Bousbih, and R. Chtourou, “Influences of the iron ion (Fe^{3+})doping on structural and optical properties of nanocrystalline TiO_{2} thin films prepared by solgel spin coating,” Applied Surface Science, vol. 257, no. 24, pp. 10699–10703, 2011. View at: Publisher Site  Google Scholar
 Y. Yalçin, M. Kiliç, and Z. Çinar, “Fe^{+3}doped TiO_{2}: a combined experimental and computational approach to the evaluation of visible light activity,” Applied Catalysis B, vol. 99, no. 34, pp. 469–477, 2010. View at: Publisher Site  Google Scholar
 X. Hou, M. Huang, X. Wu, and A. Liu, “Firstprinciples calculations on implanted TiO_{2} by 3d transition metal ions,” Science in China, Series G, vol. 52, no. 6, pp. 838–842, 2009. View at: Publisher Site  Google Scholar
 Y. Su, Y. Xiao, Y. Li, Y. Du, and Y. Zhang, “Preparation, photocatalytic performance and electronic structures of visiblelightdriven FeNcodoped TiO_{2} nanoparticles,” Materials Chemistry and Physics, vol. 126, no. 3, pp. 761–768, 2011. View at: Publisher Site  Google Scholar
 L. Jia, C. Wu, S. Han et al., “Theoretical study on the electronic and optical properties of (N, Fe)codoped anatase TiO_{2} photocatalyst,” Journal of Alloys and Compounds, vol. 509, no. 20, pp. 6067–6071, 2011. View at: Publisher Site  Google Scholar
 M. D. Segall, P. J. D. Lindan, M. J. Probert et al., “Firstprinciples simulation: ideas, illustrations and the CASTEP code,” Journal of Physics Condensed Matter, vol. 14, no. 11, pp. 2717–2744, 2002. View at: Publisher Site  Google Scholar
 D. Vanderbilt, “Soft selfconsistent pseudopotentials in a generalized eigenvalue formalism,” Physical Review B, vol. 41, no. 11, pp. 7892–7895, 1990. View at: Publisher Site  Google Scholar
 H. J. Monkhorst and J. D. Pack, “Special points for Brillouinzone integrations,” Physical Review B, vol. 13, no. 12, pp. 5188–5192, 1976. View at: Publisher Site  Google Scholar
 Z. Wu and R. E. Cohen, “More accurate generalized gradient approximation for solids,” Physical Review B, vol. 73, no. 23, Article ID 235116, 6 pages, 2006. View at: Google Scholar
 S. L. Dudarev, G. A. Botton, S. Y. Savrasov, C. J. Humphreys, and A. P. Sutton, “Electronenergyloss spectra and the structural stability of nickel oxide: an LSDA+U study,” Physical Review B, vol. 57, no. 3, pp. 1505–1509, 1998. View at: Google Scholar
 G. Shao, “Red shift in manganese and irondoped TiO_{2}: a DFT+U analysis,” Journal of Physical Chemistry C, vol. 113, no. 16, pp. 6800–6808, 2009. View at: Publisher Site  Google Scholar
 J. K. Burdett, T. Hughbanks, G. J. Miller, J. W. Richardson, and J. V. Smith, “Structuralelectronic relationships in inorganic solids: powder neutron diffraction studies of the rutile and anatase polymorphs of titanium dioxide at 15 and 295 K,” Journal of the American Chemical Society, vol. 109, no. 12, pp. 3639–3646, 1987. View at: Google Scholar
 C. Adán, A. Bahamonde, M. FernándezGarcía, and A. MartínezArias, “Structure and activity of nanosized irondoped anatase TiO_{2} catalysts for phenol photocatalytic degradation,” Applied Catalysis B, vol. 72, no. 12, pp. 11–17, 2007. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2012 HsuanChung Wu et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.